Wear, 84 (1983)
183 - 202
RESIDUAL STRESSES AND SLIDING WEAR
J. W. HO*, C. NOYAN
and J. B. COHEN
Department of Materials Science and Engineering, western University, E~~ston, IL 60201 (U.S.A.)
V. D. KHANNA and Z. ELIEZER Department of Mechanical Engineering, and Materials Science and Engineering The University of Texas at Austin, Austin, TX 78712 (U.S.A.) (Received
Summary The residual stresses that develop during the wear of AISI-SAE 1018 and 4340 steels have been examined. The entire th~~~ension~ stress tensor was obtained. A normal stress perpendicular to the surface, predicted by theory, has been found, but its magnitude is too small to affect the wear rate. There are also significant shear stresses. The wear process rapidly alters any initial stress distribution produced by heat treatment or peening to such a degree that the wear rate is not affected by these stresses, unless they are initially larger than those that can be produced by the wear parameters.
1, Introduction In recent years a new theory for sliding wear has been proposed by Suh  and his coworkers. According to this theory, cracks initiate beneath the surface and propagate parallel to the surface in a wearing material. The spread of such cracks results in the formation of lamellae which eventually separate. The cyclic loading occurring during wear contributes to crack propagation in a way similar to that in fatigue. It is well known that residual stress strongly influences fatigue behavior [Z] and, consequently, changes in residual stress during sliding might be expected to influence wear behavior. The purpose of this paper is (a) to determine the nature (the sign and the magnitude) of residual stresses induced by sliding motion and (b) to determine the influence of preexisting residual stresses on the wear behavior of steels.
*Present address: Research Institute sity, Xian, Shaanxi, China.
on Strength of Materials, Xian Jiaotong
@ Elsevier S~uoia/~~ted
in The Netherlands
Residual stresses produced in rolling contacts have been calculated by Merwin and Johnson . They assumed that, when a solid is under load, a compression normal to the surface is produced. However, the decrease in this dimension cannot occur without resistance from the part. Therefore, compressive residual stresses develop in a plane parallel to the surface to prevent further yielding. The model is simplified since both plane stress and no strain hardening are assumed. Thus, no residual stress perpendicular to the surface is considered, and all shear components are zero. Suh and coworkers have employed Merwin and Johnson’s model to calculate the residual stress distribution after sliding wear by considering a tangential force acting in the surface. The results of their calculations are shown in Fig. l(a) . It can be seen that, the higher the friction coefficient, the larger is the compressive stress ui 1 (in a plane parallel to the surface and in the direction of sliding) and the closer is its maximum to the surface. They pointed out that these residual stresses probably contribute to subsurface crack initiation in two-phase materials. However, these stresses would not influence crack propagation in a plane parallel to the surface. Therefore, when crack propagation is much slower than crack initiation, residual stresses should have little effect on the wear rate. Recently, Chiu [ 51 reconsidered the case of rolling contact, taking into account strain hardening during plastic deformation. His calculations (for AISI-SAE 52100 at a hardness level of 58.5 HRC, under a pressure of 3.85 GPa) are shown in Fig. l(b). A tensile stress perpendicular to the surface,
Depth below surface
Fig. 1. (a) Residual stresses produced by sliding wear (p, loading stress;k, yield strength in shear; ~1, friction coefficient;~, depth from the surface;a, half the contact length of an asperity) (from ref. 4); (b) residual stresses produced by rolling contact (y, depth from the surface; a, half the contact length; u33 and u1 r, stresses perpendicular to the surface and parallel to the work track respectively) (from ref. 5).
os3 t exists at a certain depth from the surface. Chiu suggested that this residual tensile stress might contribute to crack initiation. However, while the yield strength of AISI-SAE 52100 (at 58.5 HRC) is about 3000 MPa [ 51, the calculated value of the maximum residual stress is only about 20 MPa. This value seems to be too small to affect crack initiation. Actually, experiments done using parameters similar to those used by Chiu in his calculations showed  that oll and uzz can reach about 800 - 1000 MPa. If 033 was comparable with these values, it would indeed affect the wear rate. It is evident that an experimental determination of cr33 would be of considerable interest. The effect of cl1 and oz2 on the wear rate is still unclear. Some researchers [ 7, 8 J conclude that, as the compressive residual stresses (al1 and/or oz2) increase, the wear rate decreases. Unfortunately, these workers did not separate the effect of hardness from that of residual stresses. When the residual stresses are altered by either plastic deformation or heat treatment, the hardness also changes. Since the wear rate is hardness dependent, changes in the residual stresses can be expected to be correlated with changes in the wear rate under such circumstances. In order to eliminate hardness as a variable, investigators have employed a loading stress to simulate residual stress, e.g. as in ref. 9. Their results showed that, as the tensile loading stress on the sample increases, so also does the wear rate. However, residual stresses may change during wear, so the actual effect may be different from that resulting from a constant loading stress.
of the stress tensor: theoretical considerations
The stresses in surface layers can be measured by X-ray diffraction methods [lo], since they alter the shape of the interplanar spacing dq uersus sin2\Ir (Fig. 2) where \k is the angle between the normal to the surface and the normal to the diffracting planes.
Fig. 2. Geometry for X-ray diffraction measurement of stress. The interplan~ spacing was measured along L3.
The main equations for X-ray measurements of stress have recently been generalized to include the stress normal to the surface ill.]. With a subscript 3 indicating this direction, the strain eS3’ can be written as
= kll) [email protected]
sin29 + (ei2) sin 26 sin2\k + (c,,> cos $ sin 2\k + + (e22) sin2# sin29 + (fz,,) sin # sin 2* + (eaa) cos2*
(0,) and (Eij) are average values of stress and strain in the volume associated with the X-ray penetration depth, Si and S2 are elastic constants for the (Ml) planes, do is the stress-free d spacing of the (Ml) planes and $J is the angle on the surface from the principal stress axis (Fig. 2). Now let
(dw+)f &,,J _
= (eS3) + (&ii) cos2$ + Gi2) sin 24 + (s2J sin2$ - (e3s)) sin2!P
= (&is) cos C#+ (e& sin Cp)sin/2\kl
If dw+ and dew_. are measured at +\k and -9 tilts, a, and a2 can be determined. The value of (ess) is obtained from the intercept of aI uersus sin29 if do is known. The tensor components (elr), (ei2) and (e22) are obtained from aa1/a(sin2\k). For Q, = 90”, (e2,> - 6~~s) is evaluated. The tensor component (e,,> can be obtained from aa,/8(sin2\k) at rt, = 45”. From 3a2/8(sin12?lrl), &is) results when Cp= 0” and (E& when Cp= 90”. With this X-ray diffraction method, the residual stress tensor can be measured versus depth below the surface by etching. These stresses will reach a new balance after each etch. If only a small window is so etched, and the removed layer is very thin compared with the cross section of the sample, it will not appreciably perturb the initial d~tribu~on of o I 1 and ~1~~.However,
it will affect the distribution of (733,since this component is always zero at the surface, The measured value is an average over a certain depth. Once a layer has been etched away, u 33 again falls to zero at the exposed surface, regardless of its initial value at this depth before etching. One possible way to circumvent this problem is by using several X-ray wavelengths to obtain several average u33 values with different penetration depths and then to interpolate. More work has to be done to test this possibility in practice. For our purposes, to avoid this correction, we chose the wear test parameters so as to produce delamination within the X-ray penetration depth. Experiments reveal that cracks may propagate parallel to the surface at depths of about 5 grn f 123. This is just the pene~ation depth for chromium radiation in steel. The wear parameters were selected to be similar to those in ref. 12, and the depth at which cracks formed was determined by scanning electron microscopy. We shall focus on the measurement of (733 in the first layer; other values are given only to suggest the variation with depth. 3. Experimental procedures 3.1. Sample preparation Two groups of specimens were prepared, from AISI-SAE 1018 and 4340 steels. The mechanical and thermal treatments are shown in Table 1. AISI-SAE 1018 discs of 75 mm diameter were cut from 300 mm X 300 mm X 6 mm plates. After being austenitiz~ at 980 “C and quenched in ice brine, these discs were tempered at 680 “C for 2 h (all tempering was done in air). The surface was ground (under coolant) to remove the decarburized layer and polished using 600 grit emery paper. Back-reflection Debye-Scherrer rings were examined with unfiltered cobalt radiation after the surface layer had been etched off. These rings were uniform, indicating that the grain size was fine and that there was no appreciable preferred orientation. Referring to Table 1, the sample labeled A was obtained by annealing at 420 - 440 “C for 1 h under a pressure of (3 - 4) X lo_6 Torr. Specimen AS was obtained by shot peening, to induce compre~ive stresses. However, the shot-peen~g process also led to an increase in hardness. In order to separate these two factors (the residual stress and the hardness), a sample was prepared in the following way. An annealed disc was bent into a dome (of depth 2 - 4 mm), shot peened on the concave side and then flattened to release the residual stress by plastic deformation. This sample was labeled AF. Since the shot-peening intensity was the same for the AS and AF samples the resulting hardness was the same, while the residual stress pattern was different. The AISI-SAE 4340 discs (4 mm thick) were cut from a rod 50 mm in diameter. After being quenched in oil from 840 “C, the discs were tempered (at 420 - 430 “C) for 1.5 h to a hardnes of 44 HRC. Again, three sets of specimens were prepared (Table 1) : hardened (H) ; hardened and shot peened (HS); hardened, bent, shot peened and flattened (HF). Finally all specimens were polished using 600 grit emery paper.
Mechanical Specimen ~.
and thermal la be1
treatments of samples _--_..-AISI-SAE
A AW AS ASW AF
1018 1018 1018 1018 1018
H HW HS HSW HF
4340 4 340 4340 4340 4340
Vacuum annealed and polished Vacuum annealed, polished and worn Annealed, shot peened and polished Annealed, shot peened, polished and worn Annealed, bent, shot peened, flattened and polished Annealed, bent, shot peened, flattened, polished and worn Hardened and polished Hardened, polished and worn Hardened, shot peened and polished Hardened, shot peened, polished and worn Hardened, bent, shot peened, flattened and polished Hardened, bent, shot peened, flattened, polished and worn ~
The tempering temperature of the hardened sample was selected so as to eliminate residue stresses induced during quenching and yet to enable a high yield strength to be retained. The reported ultima~ tensile strength of AISI-SAE 4340 steel for tempering at 425 “C is about 1500 MPa, while the yield strength is about 1400 MPa [ 131. Because of this small difference between the ultimate tensile strength and the yield values, plastic deformation is limited. The hardness of the shot-peened sample is similar to that after tempering, while the residual stress distribution is quite different. 3.2, Wear tests Sliding wear was carried out on a pin-on-disc type of machine [ 141. All experiments were performed in air, at ambient pressure and temperature. The cylindrical pin was made of a hardened AISI-SAE 01 tool steel and had a diameter of 6.35 mm. The friction force was measured with a strain ring while the wear of the disc was obtained with a linear v~iable~isplacement transducer (LVDT). The pin displacements were read from the recorder chart and plotted as a function of time. From such plots, via a least-squares regression procedure, the steady state wear rate of the disc was determined. For the hardened discs the wear rates were calculated from the LVDT measurements and also from weight loss. The experimental parameters employed in all wear tests are given in Table 2. 3.3. Measurements of residual stress by X-rays A Picker diffractometer (equipped with a quarter-circle goniometer), a sc~ti~ation detector and a pulse height analyzer were employed. The divergence slit and receiving slit were 1” and 0.4” respectively. The irradiated
Load(N) Velocity (m s-l) Diameter of track (mm)
9.62 0.15 50
22.3 0.069 35
spot on a specimen was limited (with lead at the divergence slit) to 2 mm X 2 mm to keep the X-ray beam on the worn track, even at high \k tilt angles. Chromium radiation was employed to examine the (211) peak. For each of the $ angles of O”, 45” and 90”, 11 \E tilts were chosen: O”, -+18.43”, +26.57”, ?33.21”, k39.23” and _+45”. The 4 tilts were made about an axis parallel to the plane of diffraction; 9 was about an axis normal to this plane. Altogether, 33 peaks were examined to solve eqn. (1) by least squares for the six strain components. All the experimental data were accumulated and analyzed with the aid of a DEC PDP 8/E minicomputer. The elastic constants employed in the data analysis were calculated from single-crystal compliances according to Kroner’s theory of bulk elasticity, which assumes an anisotropic crystal coupled to isotropic surroundings [ 15,161: Si(211) i&(211)
= 0.577 X lo-’
Special consideration was given to the following: (i) Ko doublet correction; (ii) angle-dependent intensity corrections; (iii) sample alignment; (iv) stressfree lattice parameter; (v) effects of stress gradient. 3.3.1. Kcu doublet correction Because a stationary receiving slit was employed, the Kar-Ka, doublet resolution varied from the annealed to the shot-peened specimens, and with the various \k tilts. The apparent peak position of the Ka, radiation is influenced to some extent by the Kcu, component, depending on the width of the profile. For Cr Ka and the (211) peak a correction was applied if the halfwidth was broader than about 1.4” [ 171. 3.3.2. Angle-dependent intensity corrections Intensities were corrected for the Lorentz polarization and absorption factors, and also for the background (which was measured at 213 = 151” for the annealed samples, and 28 = 150” for the hardened samples). After correction, the peak position was determined by a five-point parabolic fit to the top 15% of the peak.
3.3.3. Sample alignment Peak positions obtained with the stationary slit method work) are not very sensitive to sample displacement.
(employed in Nevertheless,
absolute values of the d spacing, d,*, are required in eqn. (1) for the stress tensor calculation. The sample displacement can be obtained from the slope of the lattice parameter versus the Nelson-Riley factor [ 181. A linear least-squares fit for the (llO), (220) and (211) peaks was employed. The displacement was then adjusted to within 25 pm of the center of the goniometer. (The Lorentz polarization, absorption and doublet corrections were included in the alignment procedure.) The ambient temperature was kept constant to within 2 - 3 “C. 3.3.4. Stress-free ~ttice parameter a0 The do value is impo~~t for the copulations of the normal components of the stress tensor. In these experiments, for instance, if a0 increased by 0.0001 1$, the tensile normal stresses would decrease by about 17 MPa, and the compressive normal stress would increase by an equal amount. Tempering at 420 - 430 “C is sufficient to release the macroresidual stresses of a quenched sample. The a0 values of both steels were examined on a spot which was exposed by etching to a depth of about 100 pm from the surface. First, the fresh surface was examined. If the stress was within 210 MPa, the sample was realigned to reduce the displacement to 10 pm. Then measurements were made at all 33 values of Cp,\k. The value of a0 was determined from the average of these 33 peak positions: annealed AISI-SAE 1018 sample, 2.866 40(5) 8; hardened and tempered AISI-SAE 4340 sample, 2.867 60(Q) 8. The values in parentheses represent the errors. 3.3.5. Effects of stress gradient The effects of the stress gradient and layer removal were estimated. The effects of stress gradient altered the stresses by 10% or less. The layer removal caused a change of only about 2%, with the assumption that an entire layer was removed. As only a window was removed, the effect is even smaller. 3.4. Hardness tests
The Vickers hardness of annealed AISI-SAE 1018 samples was determined from an average of six readings taken with a load of 50 gf. For the hardened AISI-SAE 4340 samples, the average of at least 12 readings was employed, with a 100 gf load. The hardness variation versus depth was determined by etching with the same solution as used in the measurements of the stress distribution, namely 200 parts 30% HzOz and 15 parts 48% HF, contained in an ice-water bath. 4. Results and discussion
4.1. Annealed samples (AISI-SAE 1018) Before wear, the annealed samples contained fairly low residual stresses (Fig. 3) which probably were induced by cooling after the v~uum anneal.
Fig. 3. Residual stresses iu AISI-SAE 1018 steel prior to wear for (a) sample A (annealed), (b) sample AS (annealed and shot peened) and (e) sample AF (annealed, bent, shot peened and flattened): 0, @11; 0, uzz;A, 0~3.
Fig. 4. Vickers hardness of AISI-SAE 1018 steel: (a) samples A (A) and AW (+);(b) ples AS (A) and ASW (+);(c) samples AF (A) and AFW (+).
Fig. 5. Crack under worn track. The sample was pIated with electroless nickel prior to sectioning.
The AS sample (annealed and shot peened) displays compressive stresses oll and 022 of equal magnitude (Fig. 3(b)). The distribution uersus depth is typical after shot peening. Sample AF (annealed, bent, shot peened and flattened) exhibits quite a different distribution from that for AS, for both ori and oz2 (Fig. 3(c)). The value of oil is zero at a depth of about 25 pm. The large compressive value for oil at the surface is due to polishing (performed in order to obtain the same initial roughness for all samples), The value of u22, which is probably less important than ull for wear resistance, remains compressive for large depths but its value is smaller than in sample AS. The stress component 033 and the shear components are nearly zero in these three samples. Before wear, the hardness distributions in the AS and AF samples are similar, but different from that in sample A (Fig. 4). After wear, cracks were found in a drastically deformed layer within about 10 pm beneath the surface (Fig. 5). The value of 023 in this layer is tensile (in agreement with expectations), but its magnitude is only about 40 MPa, much smaller than that of cl1 or 022 (Fig. 6). By comparison of Figs. 3(a) and 6(a) it can be seen that ull and ~12~ change their distribution with wear, but only over a depth of about 75 ym. Within this depth the distributions of or, and u22 in the worn track are similar for all worn samples, and so are the hardness distributions (Fig. 4). The wear rates were calculated under steady state conditions. Usually, this required a couple of hours to attain. In order to discover how soon the final residual stress pattern develops, measurements were made on a worn track after only 100 revolutions. The similarity between Fig. 7 and Fig. 6(a) shows that the final pattern is established in only a few minutes of wear. Shear stresses in the worn track are not significant, except for c13. Frgure 8 shows that (713has a maximum value of about -35 MPa at the surface and decreases through the depth. The negative sign indicates that the shear residual stress is opposite to the direction of motion of the pin. In order to compare the magnitudes of the residual and loading stresses, the contact stress between two flat surfaces has been evaluated following
DEPTH (MCRONS) 2007
A A A 0
Fig. 6. Residual stresses in AISI-SAE 1018 steel after wear for (a) sample AW (sample A, after wear), (b) sample ASW (sample AS, after wear) and (c) sample AFW (sample AF, after wear): •,~~l;o,o~~;A,a~~.
” A A O-.
DEPTH (%RON~ Fig. 7. Residual stresses under the worn track of sample A after 100 revolutions: 0, Q22iA, (533.
5Q A +
Fig. 8. Shear residual stress ~$3 on sample A: 0, AW; 0, ASW; A, AFW; +, AlOOW.
Greenwood and Tripp [ 19f. When parabolic asperities with a height distribution close to gaussian are brought into contact with a flat surface in the absence of any tangential force, the total number of contacts, N(d), can be expressed as N(d) = 47r([email protected]
)qAF ; 0 where q, /3 and o are the density, tip radius of curvature and standard deviation (of peak height) of the asperities respectively. Here, @a is an empirical number known to be about 0.05, A is the apparent area of contact, d is the apparent distance between asperities and ~(d/~) depends on the nominal pressure and takes a value of 0.02’7 [ 191 at a pressure of 3.15 kgf cm-2. If q
and (I are assumed to be 2000 mmW2 and 5 X lo-” mm respectively, N(d) is 1150. By distributing the loading force over the number of contacts, N(d), the hertzian stress was estimated. Its value u,,, was about 1300 MPa at a depth of about 1.8 pm. If the tangential stress were taken into account, the shear stress could be as large as 0.4~,,, within 1 pm, and for a friction coefficient larger than 0.4. The facts that the residual stresses tend to be identical in the worn surfaces independent of their initial distribution and that their magnitude is much lower than that of the loading stress explain why the wear rates of all the annealed samples are similar (Table 3). TABLE
and wear values for AISI-SAE
Temperature (“C) Relative humidity (%) Friction coefficient Wear rate (mm3 km-*)
1018 samples Sample A
23.3 64 0.566 0.239
23.3 64 0.564 0.285
23.3 64 0.572 0.297
4.2. Hardened samples fAISI--SAE 4340) Before wear, the residual stress distributions in samples H and HS were different (Figs. 9(a) and 9(b)), The bending process did not significantly change uii or u33 (Fig. 9(c)); plastic deformation was limited in this springleaf-like sample. The hardness values were essentially the same for all three hardened samples before and after wear, and through the depth (Fig. 10). The distribution of residual stresses after wear (Fig. 11) shows that the depth influenced by wear was only about 25 pm, much less than that in the annealed samples. The value of es3 was about 50 MPa on the surface, while the shear stresses (Fig. 12) were in the approximate range 125 - 175 MPa. The wear rates and the friction coefficients of the hardened samples are higher than those after shot peening (Table 4). As their hardness is the same (Fig. 10(a)), this difference probably results from the different initial stress distributions in these samples. In the hardened sample (H) the wear process changes the initial stress distribution, inducing large compressive uii and ozz components near the surface. In sample HS, however, the stress distribution after wear is hardly distinguishable from the initial one; perhaps, the large initial ull and u22 values prevent deformation in the surface layer, thus resulting in a low wear rate. In a study on the relationship between delegation wear and fatigue cracks, Ritchie 1201 suggested that wear rates correlate with microcracks,
2 d v)
DEPTH (MICRONS) (b)
(4 Fig. 9. Residual stresses in AISI-SAE 4340 quenched and tempered to 44 HRC for (a) sample H, (b) sample HS (quenched, tempered to 44 HRC and shot peened) and (c) sample HF (quenched, tempered to 44 HRC, bent, shot peened and ffattened): 0,011; 0, f722iA,fT33.
Fig. 10. Vickers hardness of AISI-SAE 4340 steel: (a) samples HSW (0); (b) samples HF (A) and HFW (+).
HW (+), HS
and not with macrocracks. It is possible that the hardened two-phase material is somewhat more homogeneous after shot pee&g, thus preventing the propagation of microcracks; in such a case, a lower wear rate would also result. In general the friction coefficient depends on the same type of pararneters as the wear rate 1211. Accordingly, the difference between the friction coefficients of the H and HS samples can be explained along the same lines.
i. -6OO-- 93 (,
ZOO7 A A
-ooo-.EimD 07 m
-,ooolp 0 20
DEPTH (MICRONS) (cl Fig. 11. Residual stresses in AISI-SAE 4340 steel after wear for (a) sample HW (sample H, after wear), (b) sample HSW (sample HS, after wear) and (c) sample HFW (sample HF, after wear): 0, u~l;O, 022;C,~33.
Fig. 12. Shear stresses
u13 in worn AISI-SAE
and wear values for AISESAE
Temperature (“C) Relative humidity (%) Friction coefficient Wear rate ( mm3 km-‘)
4340 steel; 0, HW;o,
23.3 40 0.785 0.011
23.3 40 0.813 0.012
24.4 58 0.583 0.00284
23.2 37 0.68 0.00117
5. Conclusions (1) Although a residual stress component normal to the surface, (Tag, does exist in a worn surface, its magnitude is much lower than that for ull and c22. It is unlikely that it would affect the wear rate to a significant extent. (2) The only shear stress which is appreciable in a worn surface is u13. Its maximum values are about 35 MPa and 125 - 175 MPa for annealed and hardened samples respectively. Its direction is opposite to the pin motion direction. As such, it may contribute to crack propagation. (3) Residual stresses build up in the early stages of wear and any initial stress pattern is destroyed. This is true for both the annealed and the hardened steel, with the exception of the hardened and shot-peened sample. In this latter specimen the initial o,i and oz2 values were larger than could eventually be induced by the sliding action under our experimental conditions.
(4) Because the sliding action changes residual stresses to a common pattern, the wear rate is virtually independent of the initial stress distribution, unless the initial stress pattern involves values larger than those produced by wear. Acknowledgments This research was supported at Northwestern University by the Office of Naval Research, and at The University of Texas by the Houston Lighting and Power Company. The joint effort was initiated while one of the authors (J.B.C.) was a visiting professor at The University of Texas. Sample preparation, X-ray measurements and hardness testing were carried out at Northwestern University, the former in the X-ray diffraction facility of Northwestern’s Materials Research Center, supported in part by the National Science Foundation under Grant DMR-76-80847. The authors thank the Metal Improvement Company for carrying out the shot peening. References 1 N. P. Suh, An overview of the delamination theory of wear, Wear, 44 (1977) 1 - 16. 2 J. 0. Almen and P. H. Black, Residual Stresses and Fatigue in Met&, McGraw-Hill, New York, 1964. 3 J. E. Merwin and K. L. Johnson, An analysis of plastic deformation in rolling contact, Proc., Inst. Mech. Eng., London, 177 (1963) 676 - 690. 4 S. Jahanmir and N. P. Suh, Mechanics of subsurface void nucleation in delamination wear, Wear, 44 (1977) 17 - 38. 5 Y. P. Chiu, On the plastic growth and residual stresses due to contact load applied in two stages, Solid Contact and Lubrication, AMD, 39 (1980) 193 - 204. 6 H. Muro, N. Tsushima and K. Nundme, Failure analysis of rolling bearings by X-ray measurement of residual stress, Wear, 25 (1973) 345 - 356. 7 T. Sasaki, T. Yamada and K. Hatano, A study on the stress induced in the sliding surface of hardened 0.4%C steels under a dry condition, J. Jpn. Inst. Met., 38 (1974) 599 - 603 (in Japanese). 8 T. Yamada and T. Sasaki, A study on wear characteristics and the stress induced in the sliding surface of hardened steel under dry conditions, J. Jpn. Inst. Met., 39 (1975) 1199 - 1204 (in Japanese). 9 K. Endo, Y. Fukuda and G. Inoue, Influence of internal stresses on the wear of steel, Precis. Mach., 37 (1971) 496 - 501 (in Japanese). 10 B. D. Cullity, Elements of X-ray Diffraction, Addison-Wesley, Reading, MA, 1978, pp. 447 - 479. 11 H. Dolle, Influence of multiaxial stress states, stress gradients and elastic anisotropy on the evaluation of stress by X-rays, J. Appl. Crystallogr., 12 (1979) 489 - 501. 12 N. Saka, A. M. Eleiche and N. P. Suh, Wear of metals at high sliding speeds, Wear, 44 (1977) 109 - 125. 13 T. Baumeister and E. A. Avallone (eds.), Mark’s Standard Handbook for Mechanical Engineers, McGraw-Hill, New York, 8th edn., 1978. 14 V. D. Khanna, Effect of thermoelectric current on the friction and wear behavior of an iron-constantan couple, Master’s Thesis, The University of Texas at Austin, 1977. 15 E. Kroner, Elastic moduli of perfectly disordered composite materials, J. Mech. Phys. Solids, 15 (1967) 319 - 329. 16 G. Simmons and H. Wang, Single Crystal Elastic Constants and Aggregate Properties,
202 Massachusetts Institute of Technology Press, Cambridge, MA, 1971. 17 J. B. Cohen, H. Dolle and M. R. James, Determining stresses from X-ray powder patterns, Symp. on Accuracy in Powder Diffraction, in NBS Spec. Publ. 567, February 1980, pp. 453 - 477 (National Bureau of Standards, U.S. Department of Commerce). 18 L. H. Schwartz and J. B. Cohen, Diffraction from Materials, Academic Press, New York, 1977, pp. 245 - 246. 19 J. A. Greenwood and J. H. Tripp, The contact of two nominally flat rough surfaces, Proc., Inst. Mech. Eng., London, 185 (1971) 625 - 633. 20 R. 0. Ritchie, On the relationship between delamination wear and the initiation and growth of fatigue cracks in ultrahigh strength steel. In N. P. Suh and N. Saka (eds.), Fundamentals of Tribology, Massachusetts Institute of Technology Press, Cambridge, MA, 1978, pp. 127 - 134. 21 N. Saka, Effect of microstructure on friction and wear of metals. In N. P. Suh and N. Saka (eds.), Fundamentals of Tribology, Massachusetts Institute of Technology Press, Cambridge, MA, 1978, pp. 135 - 170.